The host response to calcium silicate ceramic coatings is not always favorable because of their high dissolution rates, leading to high pH within the surrounding physiological environment. Recently, a zinc-incorporated calcium silicate-based ceramic Ca2ZnSi2O7 coating, developed on a Ti-6Al-4V substrate using plasma-spray technology, was found to exhibit improved chemical stability and biocompatibility. This study aimed to investigate and compare the in vitro response of osteoblastic MC3T3-E1 cells cultured on Ca2ZnSi2O7 coating, CaSiO3 coating, and uncoated Ti-6Al-4V titanium control at cellular and molecular level. Our results showed Ca2ZnSi2O7 coating enhanced MC3T3-E1 cell attachment, proliferation, and differentiation compared to CaSiO3 coating and control. In addition, Ca2ZnSi2O7 coating increased mRNA levels of osteoblast-related genes (alkaline phosphatase, procollagen α1(I), osteocalcin), insulin-like growth factor-I (IGF-I), and transforming growth factor-β1 (TGF-β1). The in vivo osteoconductive properties of Ca2ZnSi2O7 coating, compared to CaSiO3 coating and control, was investigated using a rabbit femur defect model. Histological and histomorphometrical analysis demonstrated new bone formation in direct contact with the Ca2ZnSi2O7 coating surface in absence of fibrous tissue and higher bone-implant contact rate (BIC) in the Ca2ZnSi2O7 coating group, indicating better biocompatibility and faster osseointegration than CaSiO3 coated and control implants. These results indicate Ca2ZnSi2O7 coated implants have applications in bone tissue regeneration, since they are biocompatible and able to osseointegrate with host bone.
Citation: Yu J, Li K, Zheng X, He D, Ye X, Wang M (2013) In Vitro and In Vivo Evaluation of Zinc-Modified Ca–Si-Based Ceramic Coating for Bone Implants. PLoS ONE 8(3): e57564. https://doi.org/10.1371/journal.pone.0057564
Editor: Wei-Chun Chin, University of California, Merced, United States of America
Received: July 31, 2012; Accepted: January 24, 2013; Published: March 6, 2013
Copyright: © 2013 Yu et al. This is an open-access article distributed under the terms of the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original author and source are credited.
Funding: This work was supported by the National Natural Science Foundation of China (Grant No. 81071455) and the Fund for Key Science and Technology Program of Shanghai Science and Technology Committee (Grant No. 09441900106). The funders had no role in study design, data collection and analysis, decision to publish, or preparation of the manuscript.
Competing interests: The authors have declared that no competing interests exist.
In recent years, calcium silicate-based ceramics have become more promising as potential implant biomaterials for bone tissue engineering due to their bioactive and biocompatible properties –. Despite the beneficial influence on bone response, well-known drawbacks associated with this material exist, such as poor mechanical properties, which limit the scope of its clinical application –. However, these limitations can be overcome by surface-modification techniques , . The bioactive ceramic coating would confer adequate bioactivity to the surface of the implant, preventing direct contact between the substrate and surrounding bone tissue, thus reducing release of problematic ions from the metallic substrate.
Several coating techniques have been developed and include flame spraying, sputtering, electrophoretic coating, hot isostatic pressing and solution coating . Each approach has its advantages and disadvantages; however, plasma-spraying has shown the most promise as a coating method. In fact, plasma-spraying is reported as the method of choice for coating CaSiO3 and Ca2SiO4 onto metal substrates, both of which have been used clinically to enhance bioactivity and bonding strength with titanium alloy in comparison to HA coating . However, major limitations of calcium silicate coatings include deleterious biological effects due to their high dissolution rate and induction of high pH within the surrounding tissues, which limits further their biomedical application .
Recently, ion-modification of Ca–Si-based ceramics has been developed to improve their chemical stability and biomedical properties and includes divalent (Mg , Zn ,  and Sr ) and tetravalent (Ti  and Zr ) modification. Moreover, Ti and Zr-incorporated Ca–Si-based ceramics have been used as stable coatings that improve biomedical properties compared with calcium silicate coatings , . However, Zn-modified calcium silicate (Ca2ZnSi2O7) ceramic coatings have not been fully investigated to date. It is well established that zinc, an essential trace element, plays an important role in various physiological processes . Zn has been shown to have a stimulatory effect on bone formation and an inhibitory or biphasic effect on osteoclastic bone resorption . Zinc deficiency results in the arrest of bone growth, bone development, and the overall maintenance of bone health , . This indicates Ca2ZnSi2O7 is an interesting biomaterial coating that warrants further investigation. In our previous work, Zn was selected for incorporation into a Ca–Si system to form hardystonite (Ca2ZnSi2O7), which was used as a feedstock coating on the Ti-6Al-4V substrate using plasma-spray technology. Ca2ZnSi2O7 coating exhibited chemically stable (low dissolution) and good bioactivity in comparison with CaSiO3 coating . In the present study, we investigate how Ca2ZnSi2O7 coating affects adhesion, morphology, orientation, proliferation and osteoblast differentiation of MC3T3-E1 osteoprogenitor cells (Fig. 1a). The in vivo osseointegration potential of Ca2ZnSi2O7 coating was also assessed using a rabbit femur defect implantation model (Fig. 1b).
(b) Schematic illustration of in vivo analysis. White arrows indicated new bone was formed at the Ca2ZnSi2O7 coating periphery with direct contact to the implant surface in absence of a connective tissue layer in group 3. In contrast, a wide band of fibrous tissue was clearly seen around the surface of the CaSiO3 coating and control in group 2 and 1. Group 1, control; Group 2, CaSiO3 coating; Group 3, Ca2ZnSi2O7 coating.
Materials and Methods
Specimen Preparation and Characterization
Ca2ZnSi2O7 powders and coatings were prepared according to methods described previously . Briefly, Ca2ZnSi2O7 powders were synthesized by the sol-gel method using zinc nitrate hexahydrate (Zn(NO3)2.6H2O; Sinopharm Chemical Reagent Co., Ltd (SCRC), China), calcium nitrate tetrahydrate (Ca(NO3)2.4H2O; SCRC, China) and tetraethyl orthosilicate (TEOS, (C2H5O)4Si); SCRC, China). The obtained Ca2ZnSi2O7 powders were sieved through 80 meshes and sprayed onto Ti-6Al-4V substrates with dimensions of 10×10×2 mm and ø10×1 mm, for in vitro cell culture and in vivo study respectively. The atmosphere plasma spray (APS) system (Sulzer Metco, Switzerland) was used to fabricate all coatings. The thickness of the coating was approximately 170 µm. Before plasma-spraying, substrates were ultrasonically cleaned in acetone and grit-blasted using corundum sand of F60 grade. CaSiO3 coatings were prepared using the same conditions as the control. Samples were ultrasonically cleaned and sterilized in acetone, ethanol and distilled water for 10 min.
The phase composition, surface morphology, surface roughness (Ra) and bonding strength of the Ca2ZnSi2O7 coating was characterized in our previous work .
In vitro Testing
The osteoblast-like cell line, MC3T3-E1, was obtained from the Chinese Academy of Sciences Cell Bank. Cells were cultured in culture plates containing alpha-minimal essential medium (α-MEM, Gibco BRL, Invitrogen, Life Technologies, USA) supplemented with 10% (v/v) fetal bovine serum (FBS) and 1% (v/v) of a 100 U/ml penicillin and 100 µg/ml streptomycin solution (Gibco BRL, respectively). Cells were incubated at 37°C in the presence of 5% CO2. On reaching 80% confluence, cells were detached every 2–3 days using 0.25% trypsin/EDTA solution (Gibco BRL).
Cell attachment and morphology.
MC3T3-E1 cells were seeded onto uncoated Ti-6Al-4V titanium (control), CaSiO3 and Ca2ZnSi2O7 coated substrates within individual wells of 24-well culture plates at a density of 1×104 cells/cm2. Cells were incubated in α-MEM culture medium supplemented with 10% FBS at 37°C in 5% CO2 for 24 h. Samples were rinsed with PBS (pH 7.4) to remove non-adherent cells and fixed in 4% paraformaldehyde for 1 h. Cells were subsequently rinsed with PBS buffer containing 4% (w/v) sucrose and post-fixed in 1% osmium tetroxide in PBS, followed by sequential dehydration in an ethanol series of 30%, 50%, 70%, 90%, 95% and 100% for 5 minutes in each concentration. Specimens were sputter-coated with gold and the morphological characteristics of the attached cells were determined using scanning electron microscope (SEM, S-4800, Hitachi, Japan).
Cell proliferation was measured using a standard methyl thiazolyl tetrazolium (MTT) assay (Sigma-Aldrich, Saint Louis, MO, n = 6 for each sample). MC3T3-E1 cells were cultured on control, CaSiO3 and Ca2ZnSi2O7 coated substrates placed individually in a 24-well culture plate at a density of 1×104 cells/cm2 and allowed to grow for 1, 4, 7 and 14 days. At the specified time-points, the substrates were washed in PBS and transferred to another new 24-well plate. MTT stock solution (10% of total volume) was added to 24-well plates containing the coatings and incubated for 4 h at 37°C and 5% CO2. Medium was withdrawn and dimethyl sulphoxide (Sigma–Aldrich) was added to each well to dissolve the formazan dye crystals. 100 ul of the reacted reagent from each well was transferred to 96-well plates and the absorbance measured using a microplate reader (SPECTRA MAX PLUS 384 MK3, Thermo Fisher Scientific, Waltham, MA, USA) at a wavelength of 490 nm.
Cell differentiation and mineralization.
MC3T3-E1 cell osteoblast differentiation and mineralization were determined using cells (1×104 cells/cm2) cultured in triplicate (n = 3) on each coating group in differentiation medium comprising α-MEM medium supplemented with 50 µg/ml ascorbic acid (Sigma-Aldrich) and 10 mM β-glycerophosphate (Sigma-Aldrich). Cell differentiation and mineralization were characterized from alkaline phosphatase (ALP) activity and Osteocalcin (OC) secretion. Concentrations of ALP and OC were individually determined using ELISA kits (R&D Systems, Minneapolis, MN, USA) as described below.
Quantitative measurement of ALP activity.
MC3T3-E1 cells were cultured on control, CaSiO3 and Ca2ZnSi2O7 coated substrates in differentiation medium for 1, 4, 7 and 14 days. ALP activity was measured using stable p-nitrophenol phosphate substrate. At each time point, culture medium was removed by decantation and cells were washed with PBS and harvested in 1 ml universal ALP buffer (100 mM citric acid, 100 mM KH2PO4, 100 mM sodium tetraborate.10 H2O, 100 mM Tris, 100 mM KCl; pH 11). Cells were sonicated twice for 20 sec and centrifuged at 3000 rpm for 5 min at 4°C. ALP activity in the supernatants was determined following addition of p-nitrophenyl phosphate substrate and the reaction was stopped using 100 µl of 0.1 N NaOH. The optical density was measured at 405 nm using a microplate reader (SPECTRA MAX PLUS 384 MK3, Thermo). The ALP activity was calculated from a standard curve after normalization to total protein content, which was measured using the Bradford protein assay kit (Pierce, Rockford, IL, USA). ALP experiments were repeated twice with n = 3 for each substrate.
Quantitative measurement of OC secretion.
MC3T3-E1 cells were cultured on control, CaSiO3 and Ca2ZnSi2O7 coated substrates in differentiation medium for 1, 7, 14 and 21 days. Quantitative levels of OC secreted into the culture medium were determined using an enzyme-linked immunoassay (ELISA) kit (R&D) following the manufacturer’s instructions.
Quantitative reverse transcription-PCR (qRT-PCR).
Total RNA was isolated from MC3T3-E1 cells on each coated substrate using Trizol reagent (Fermentas, Maryland, NY, USA). First-strand cDNA synthesis was carried out using Superscript III reverse transcriptase (Invitrogen, Carlsbad, CA, USA) for 60 min at 50°C. Quantitative RT-PCR for MC3T3-E1 cell osteoblast-related genes of alkaline phosphatase (ALP), procollagen α1(I) (Col α1(I)), osteocalcin (OC)and growth factors gene of insulin-like growth factor-I (IGF-I) and transforming growth factor-β1 (TGF-β1), was performed using the ABI PRISMs 7000 Sequence Detection System (Applied Biosystems, Foster City,CA, USA). The amount of target gene transcript in each sample was determined using SYBR® Premix Ex Taq™ II (Takara, Kyoto, Japan) in a final volume of 20 µl containing the same amount of RT product (50 ng cDNA), 10 µl of 2×SYBR® Premix Ex Taq™ II and 0.8 µl of 10 µM forward and reverse primers. Primers for the selected genes are listed in Table 1. Amplification conditions were as follows: Stage 1∶95°C for 30 s; Stage 2∶30 repetitions of 95°C for 5 s, 60°C for 30 s. Each RT-PCR quantification experiment was performed in triplicate for individual samples. Final results were reported as the relative expression normalized with transcript level of the housekeeping gene, Glyceraldehyde 3-phosphate dehydrogenase (GAPDH).
In vivo Analysis
Total nine White New Zealand rabbits (obtained from Shanghai Jiao Tong University, Laboratory Animal Center, male, 2–2.5 kg body weight) were randomly divided into 3 groups. The use of animals and the experimental protocols was approved by the Institutional Animal Welfare Committee of Shanghai Jiao Tong University. A total of six cylindrical implants of approximately 1 mm in diameter and 1 cm in length were implanted into the femur of each rabbit. Three implants were inserted into the femur of the left hind leg and another three into the femur of the right hind leg. A schedule was prepared to ensure equal placement of the three implant types within each of the six femoral sites and one of each implant types placed into each femur. Rabbits were anesthetized by injecting 3% Nembutal (30 mg/kg) via the ear vein and a longitudinal incision was made by scalpel in the rabbit femur under rigorous aseptic conditions. Circular holes, 1 mm diameter by 1.0 cm deep, were drilled using a surgical electronic drill and thoroughly rinsed with physiological saline to remove shards of bone. Implants of Ti–6Al–4V (control), CaSiO3-coated Ti–6Al–4V and Ca2ZnSi2O7-coated Ti–6Al–4V were used in this study. Before insertion of implants, blood was removed using sterile cotton balls and the holes were manually filled with implants as tightly as possible. The wound was sutured with nylon thread. Rabbits were sacrificed 1.5 month after implantation.
After sacrifice, Excised specimens were fixed in 4% paraformaldehyde for 3 days, dehydrated in a series of ethanol solutions (70, 80, 90, 95 and 100%) and embedded in polymethylmethacrylate resin. Undecalcified sections with a thickness of 100 µm were cut using a saw microtome (Leica ST1600) and stained with trinitrophenol-fuchsin prior to histological analysis. A minimum of 6 sections were made from each implant and used for descriptive and morphometric analyses.
Histology and histomorphometry.
Histological observation and histomorphometrical analysis of the sections were performed under a biologic fluorescence microscope (Olympus BX-60). The microscopic images of the sections were digitized and analyzed using an image-analyzing software (KS400). The bone-implant contact rate (BIC) was used as the index of osseointegration, equal to the surface length contact of the implant with the bone/the overall surface length of implant inserted into the bone.
For statistical analysis, first Levene’s test was performed to determine the homogeneity of variance for all the data, and then one way analysis of variance followed by Tukey or Tamhane’s T2 post-hoc test for multiple comparison was performed for the comparisons between different groups. SPSS 17.0 program was employed for all statistical analysis and differences were considered significant if p<0.05. All data were expressed as a mean ± standard deviation (SD).
Cell Attachment and Morphology
MC3T3-E1 cell attachment and morphology on control, CaSiO3 and Ca2ZnSi2O7 coated substrates were examined using SEM (Fig. 2). After 24 h of culture, MC3T3-E1 cells were found to attach to all tested samples surface. The cells displayed a triangle-like morphology on the surface of the titanium control (Fig. 2a, b) but appeared spindle-like on the surface of both the Ca2ZnSi2O7 (Fig. 2e, f) and CaSiO3 (Fig. 2c, d) coated substrates. A greater number of cells had cytoplasmic extensions, which were longer in protrusion, on the Ca2ZnSi2O7 coated surface in comparison to CaSiO3 and control.
MC3T3-E1 cell proliferation on control, CaSiO3 and Ca2ZnSi2O7 coated substrates was determined using an MTT assay. A statistically significant increase in cell proliferation was measured on all samples with increasing culture time (Fig. 3). Cell proliferation was increased on days 1, 4, 7 and 14 on Ca2ZnSi2O7 coated substrate compared to either CaSiO3 coated substrate or control (p<0.05).
Cell proliferation of MC3T3-E1 cells cultured on the different substrates was measured by MTT assay. Ca2ZnSi2O7 coating enhanced the proliferation of preosteoblasts. All experiments were repeated in triplicate *Ca2ZnSi2O7 coating compared with CaSiO3 coating or control, p<0.05. Data presented as mean ± SD (n = 6).
Cell Differentiation and Mineralization
Cell differentiation from pre-osteoblasts to osteoblasts revealed osteogenic functioning of MC3T3-E1 cells on all substrates. ALP assays were performed on MC3T3-E1 cells cultured on control, CaSiO3 and Ca2ZnSi2O7 coated substrates at various time points. ALP activity presented a similar profile for all samples, with increased activity throughout the culture duration (Fig. 4). For all conditions tested, there was no significant difference in ALP activity between days 1 and 4, after which levels rapidly increased up to day 14. ALP activity within cells incubated on Ca2ZnSi2O7 coating increased above those on the CaSiO3 coating and control (p<0.05 for CaSiO3 coating and control at day 7, 14). Results therefore indicate that Ca2ZnSi2O7 coating can promote cell maturation as reflected by increased ALP activity.
All experiments were repeated twice with n = 3 for each substrate. *Ca2ZnSi2O7 coating compared with CaSiO3 coating or control, p<0.05. Results are presented as mean ± SD.
Levels of the differentiation marker, OC, were investigated at days 1, 7, 14 and 21 of culture. As shown in Fig. 5, no significant difference in OC levels were found in MC3T3-E1 cells cultured on Ca2ZnSi2O7, CaSiO3 and control substrates at day 1. However, increases in OC were observed at days 7, 14 and 21 (p<0.05) in cells grown on the Ca2ZnSi2O7 coating compared to CaSiO3 coated substrates and control.
Osteoblast-related Gene Expression
MC3T3-E1 cells were cultured for 1, 2 and 3 weeks on control, CaSiO3 and Ca2ZnSi2O7 coatings and expression of typical bone-related genes was examined using qRT-PCR (Fig. 6). ALP mRNA expression levels (Fig. 6a) in MC3T3 cells cultured on Ca2ZnSi2O7 coating steadily increased with time and were significantly higher (p<0.05) compared to cells cultured on CaSiO3 coating and control. These results are consistent with the previous ALP activity findings. procollagen α1(I) mRNA expression (Fig. 6b) decreased with time for all samples, but levels were significantly higher in cells on Ca2ZnSi2O7 coating in comparison to those on CaSiO3 coating and control (p<0.05 for CaSiO3 coating and control at week 1; p<0.05 for control alone at week 2). Osteocalcin mRNA expression (Fig. 6c) increased slightly over two weeks for all samples, after which levels rapidly increased up to week 3. In comparison to CaSiO3 coating and control, osteocalcin mRNA levels in cells grown on Ca2ZnSi2O7 coating were significantly increased (p<0.05 for CaSiO3 coating and control). IGF-I mRNA expression (Fig. 6d) increased with time for all samples although levels were significantly higher in cells grown on Ca2ZnSi2O7 coating compared to CaSiO3 coating and control (p<0.05 for CaSiO3 coating and control). TGF-β1 mRNA expression (Fig. 6e) increased with time for all samples and was significantly higher in cells grown on Ca2ZnSi2O7 coating compared to CaSiO3 coating and control (p<0.05 for CaSiO3 coating and control).
In vivo Analysis
The excellent in vitro properties of Ca2ZnSi2O7 coating led to analysis of its in vivo biocompatible properties following implantation into a rabbit femur defect model. No inflammation or other implant-associated complications were observed macroscopically or microscopically in any of the histopathology sections for the implanted Ca2ZnSi2O7 coatings throughout the experimental periods. After 1.5 month of implantation, new bone was primarily observed at the Ca2ZnSi2O7 coating periphery with direct contact to the implant surface in absence of a connective tissue layer (Fig. 7g–i). In contrast, fibrous tissue was clearly seen around the surface of the CaSiO3 coating (Fig. 7d–f) and control (Fig. 7a–c), resulting in markedly reduced bone-implant contact. New bone formation was sparse around these two implants.
(a–c) control, (b) magnification of the left white square in panel (a), (c) magnification of the right white square in panel (a); (d–f) CaSiO3 coating, (e) magnification of the bottom white rectangle in panel (d), (f) magnification of the top white rectangle in panel (d), (g–i) Ca2ZnSi2O7 coating, (h) magnification of the left white rectangle in panel (g), (i) magnification of the right white square in panel (g). FT, fibrous tissue; Im, implant; NB, new bone.
The results of the histomorphometric measures are shown in Fig. 8. The bone-implant contact rate (BIC) was 70.61±8.42% in the Ca2ZnSi2O7 coating group, which was significantly (p<0.05) higher than the values of 25.29±2.43% observed in the CaSiO3 coating group and 16.47±1.39% in the control group.
It showed the mean BIC over the total implant length. For the Ca2ZnSi2O7 group, the BIC showed significant differences compared with CaSiO3 coating and control (*p<0.05). Results presented are the mean ± SD (n = 6) of two independent experiments.
It is well-known that biomaterial physicochemical characteristics are important in tissue engineering because of their direct effect on cellular response and ultimately tissue regeneration . Surface modifications have been applied to metallic biomaterials in order to improve their wear properties, corrosion resistance, and biocompatibility , . Our previous studies have shown the Zn-modified calcium silicate (Ca2ZnSi2O7) ceramic coating exhibits significantly improved stability in physiological solution and good bioactivity, as well as high bonding strength with the titanium alloy substrate . We therefore conducted a more detailed study to examine and compare the in vitro and in vivo response of osteoblast-like MC3T3-E1 cells cultured on uncoated Ti-6Al-4V titanium (control), CaSiO3 coated and Ca2ZnSi2O7 coated substrates and investigate their capacity to conduct osteoregeneration after implantation into a rabbit femur defect model.
Biomaterial surface specifications can influence adsorption of biological molecules and, in the second stage, adsorption of cells . Hence, adequate adhesion and spreading of cells are prerequisite for the interaction of cells with their substrate, which will determine subsequent cellular activities including proliferation and differentiation. Investigation into cell attachment found that MC3T3-E1 cells adhere to Ca2ZnSi2O7 coating with greater spread and number of filopodia projections anchored to the surface than those adhering to CaSiO3 coating or control, which indicates that Ca2ZnSi2O7 coating has a good bioactive surface favorable for cell adhesion and growth with good biocompatibility.
Ideally bioactive biomaterials need to interact actively with cells and stimulate cell growth . MTT assay showed MC3T3-E1 cells could proliferate on all three samples. Furthermore, the proliferation ratio on Ca2ZnSi2O7 ceramic coating was higher than that on CaSiO3 coating or control at all time points, suggesting Ca2ZnSi2O7 coating modulates cell proliferation activity. Besides proliferation, the ability of preosteoblasts to differentiate on the biomaterials is an important stage that occurs before bone mineralization. ALP was used as a marker for early and mid-stages of osteoblast maturation and bone matrix production –. In our study, MC3T3-E1 cell ALP activity on Ca2ZnSi2O7 coating exhibited higher levels of expression than on CaSiO3 coating or control from day 7. This is in accordance with the results of ALP gene regulation, indicating Ca2ZnSi2O7 coating might possess a greater ability to stimulate preosteoblast differentiation compared to CaSiO3 coating and control. As expected, Zn ions appear to be the relevant inducers of ALP activity, since ALP is a Zn-dependent enzyme . OC is secreted solely by osteoblasts and thought to play a role in cell mineralization and calcium ion homeostasis . Our results show that Ca2ZnSi2O7 coating indeed markedly raises levels of OC over control levels at later periods in culture, which indicates their higher maturation state at this period. Further investigation into OC expression found mRNA levels followed a similar trend to OC levels, indicating that Zn-modified calcium silicate (Ca2ZnSi2O7) ceramic coating possesses a greater ability to promote osteoblast mineralization of MC3T3-E1 cells compared to CaSiO3 coating or control. Our findings are consistent with data reported by other research groups. Chesters  and Cousins  report that zinc is an essential trace element involved in diverse metabolic and cellular signaling pathways and is involved in the modulation of gene expression for proteins involved in bone formation. Ito et al also report that incorporation of zinc into calcium phosphate cement significantly promotes preosteoblast proliferation and differentiation in vitro –. More recently, Kwun et al. suggest zinc is involved in regulating the transcription of preosteoblast differentiation genes, such as Col-I, ALP, osteopontin and OC . Hence, Zn is considered to be one promising agent for enhancing the bone-forming ability of implant materials, which can be achieved by controlling the release of Zn ions. Our studies suggest that Zn ions released form Ca2ZnSi2O7 coatings might play an important role in MC3T3-E1 cell proliferation and differentiation.
In the present study, MC3T3-E1 cells were used to investigate the influence of Ca2ZnSi2O7 coating on regulation of osteoblast-associated genes: ALP, Col α1(I) and OC by qRT-PCR. These genes are major phenotypic markers for preosteoblast differentiation during bone formation . Col-I is the most abundant protein synthesized by active osteoblasts and is essential to mineral deposition, so its expression represents the start of osteoblast differentiation . Col α1(I) mRNA expression (early marker, major extracellular collagenous protein for organic matrix formation) was upregulated in cells on Ca2ZnSi2O7 coating compared to CaSiO3 coating and control. The increase was pronounced during the early stage time points, which represent the beginning of osteoblast differentiation. Similar results were observed by Ehara et al, who found that calcium phosphate compounds cultured with MC3T3-E1 cells accelerated osteoblast differentiation in the early phase and promoted matrix production . The results of this study demonstrate that at molecular level, osteoblast bone marker gene expression (ALP, Col α1(I), OC) on Ca2ZnSi2O7 coating is up-regulated, indicating Ca2ZnSi2O7 as a more favorable substrate for MC3T3-E1 cells with the potential for applications in bone tissue regeneration.
Growth factors have become an important component for tissue engineering and regenerative medicine –. In particular, IGF-I and TGF-β1 have great significance in bone tissue engineering . IGF-I has been implicated as a regulator of osteoblast abundance to maintain bone matrix by enhancing osteoblast matrix production  and regulating osteoclast bone resorption . TGF-β1 is considered another important regulator of osteoblast and osteoclast activity . It is activated by resorbing osteoclasts which in turn attenuates further bone resorption by impairing osteoclastogenesis and promoting bone formation through chemotactic attraction of osteoblasts, enhancement of osteoblast proliferation and the early stages of differentiation with production of ECM proteins (including Col-I, osteopontin, OC) . However, the effect of biomaterials on gene expressions of these factors in osteoblast cells has not been fully clarified. This study investigated mRNA expressions of IGF-I and TGF-β1 on the control, CaSiO3 and Ca2ZnSi2O7 coated substrates using qRT-PCR. We found that culture on Ca2ZnSi2O7 coating caused a significant increase in IGF-I and TGF-β1 mRNA expression in MC3T3-E1 cells, both of which are involved in the stimulation of bone formation and cell proliferation within osteoblast cells. Yamaguchi et al. also report that culture with zinc stimulates protein production of IGF-I, TGF-β1 or osteocalcin in osteoblastic MC3T3-E1 cells .
All the results obtained in vitro indicate that Ca2ZnSi2O7 coating is more favorable to the cellular activities of MC3T3-E1 cells, indicating that this coating might be suitable for bone regeneration and tissue engineering compared to CaSiO3 coating and control. The behavior of the bone tissue around Ca2ZnSi2O7 coating following implantation in rabbit femurs was also investigated. We found new bone was formed and in direct contact with the implants after 1.5 month of Ca2ZnSi2O7 coating implantation, in absence of fibrous tissue infiltration around the implant. In contrast, a wide band of fibrous tissue was clearly seen around the surface of the CaSiO3 coating and control. These observations were in line with the histomorphometrical data. Our results showed the direct bone contact with the implant (BIC) of Ca2ZnSi2O7 coating group was significantly greater than that for CaSiO3 coating and control after 1.5 month implantation. So, we concluded that Ca2ZnSi2O7 coatings have better bone integration properties after implantation, compared to CaSiO3 coating and control. This is consistent with the results obtained by Zreiqat et al., who observed that the incorporation of Sr and Zn into their Ca–Si system induced in vivo osteoconductivity at 3 and 6 weeks following implantation in tibial bone defects in rats .
Plasma-sprayed Ca2ZnSi2O7 coating enhanced MC3T3-E1 cell attachment, proliferation, differentiation and up-regulated bone marker gene expression of ALP, Col α1(I) and OC and growth factors genes of IGF-I and TGF-β1, compared to CaSiO3 coating and control. The in vivo study demonstrates further efficacy of Ca2ZnSi2O7 coating in modulating bone formation around the implant and enhancement of osseointegration in absence of fibrous tissue response. In conclusion, the biological properties observed for the investigated Ca2ZnSi2O7 coating strongly suggest it is a good candidate for orthopedic and dental implant fixation.
Conceived and designed the experiments: MYW XJY. Performed the experiments: JMY KL. Analyzed the data: XBZH DNH MYW XJY. Contributed reagents/materials/analysis tools: XBZH DNH. Wrote the paper: MYW XJY.
- 1. Siriphannon P, Kameshima Y, Yasumori A, Okada K, Hayashi S (2000) Influence of preparation conditions on the microstructure and bioactivity of α-CaSiO3 ceramics: Formation of hydroxyapatite in simulated body fluid. J Biomed Mater Res 52: 30–39.
- 2. Ni SY, Chang J, Chou L, Zhai WY (2007) Comparison of osteoblast-like cell responses to calcium silicate and tricalcium phosphate ceramics in vitro. J Biomed Mater Res Part B 80B: 174–183.
- 3. Xue W, Liu X, Zheng X, Ding C (2005) In vivo evaluation of plasma-sprayed wollastonite coating. Biomaterials 26: 3455–3460.
- 4. Siriphannon P, Kameshima Y, Yasumori A, Okada K, Hayashi S (2002) Formation of hydroxyapatite on CaSiO3 powders in simulated body fluid. J European Ceram Soc 22: 511–520.
- 5. Wu C, Ramaswamy Y, Soeparto A, Zreiqat H (2008) Incorporation of titanium into calcium silicate improved their chemical stability and biological properties. J Biomed Mater Res Part A. 86A: 402–410.
- 6. Liu XY, Chu PK, Ding CX (2004) Surface modification of titanium, titanium alloys, and related materials for biomedical applications. Mater Sci Eng R-Rep 47: 49–121.
- 7. Liu XY, Ding CX, Wang ZY (2001) Apatite formed on the surface of plasma-sprayed wollastonite coating immersed in simulated body fluid. Biomaterials 22: 2007–2012.
- 8. Liu XY, Ding CX, Chu PK (2004) Mechanism of apatite formation on wollastonite coatings in simulated body fluids. Biomaterials 25: 1755–1761.
- 9. Sun LM, Berndt CC, Gross KA, Kucuk A (2001) Material fundamentals and clinical performance of plasma-sprayed hydroxyapatite coatings: A review. J Biomed Mater Res 58: 570–592.
- 10. Liu XY, Tao SY, Ding CX (2002) Bioactivity of plasma sprayed dicalcium silicate coatings. Biomaterials 23: 963–968.
- 11. Wu CT, Chang JA, Wang JY, Ni SY, Zhai WY (2005) Preparation and characteristics of a calcium magnesium silicate (bredigite) bioactive ceramic. Biomaterials 26: 2925–2931.
- 12. Ramaswamy Y, Wu CT, Zhou H, Zreiqat H (2008) Biological response of human bone cells to zinc-modified Ca-Si-based ceramics. Acta Biomater 4: 1487–1497.
- 13. Lu HX, Kawazoe N, Tateishi T, Chen GP, Jin XG, et al. (2010) In vitro Proliferation and osteogenic differentiation of human bone marrow-derived mesenchymal stem cells cultured with hardystonite (Ca2ZnSi2O7) and β-TCP Ceramics. J Biomater Appl 25: 39–56.
- 14. Wu CT, Ramaswamy Y, Kwik D, Zreiqat H (2007) The effect of strontium incorporation into CaSiO3 ceramics on their physical and biological properties. Biomaterials 28: 3171–3181.
- 15. Ramaswamy Y, Wu C, Van Hummel A, Combes V, Grau G, et al. (2008) The responses of osteoblasts, osteoclasts and endothelial cells to zirconium modified calcium-silicate-based ceramic. Biomaterials 29: 4392–4402.
- 16. Liu XY, Ding CX (2002) Plasma sprayed wollastonite/TiO2 composite coatings on titanium alloys. Biomaterials 23: 4065–4077.
- 17. Liang Y, Xie YT, Ji H, Huang LP, Zheng XB (2010) Excellent stability of plasma-sprayed bioactive Ca3ZrSi2O9 ceramic coating on Ti-6Al-4V. Appl Surf Sci 256: 4677–4681.
- 18. Tapiero H, Tew KD (2003) Trace elements in human physiology and pathology: zinc and metallothioneins. Biomed Pharmacother 57: 399–411.
- 19. Yamaguchi M, Oishi H, Suketa Y (1987) Stimulatory effect of zinc on bone formation in tissue culture. Biochemical pharmacology 36: 4007–4012.
- 20. Hsieh HS, Navia JM (1980) Zinc deficiency and bone formation in guinea pig alveolar implants. J Nutr 110: 1581–1588.
- 21. Oner G, Bhaumick B, Bala RM (1984) Effect of zinc deficiency on serum somatomedin levels and skeletal growth in young rats. Endocrinology 114: 1860–1863.
- 22. Li K, Yu J, Xie Y, Huang L, Ye X, et al. (2011) Chemical stability and antimicrobial activity of plasma sprayed bioactive Ca2ZnSi 2O7)coating. J Mater sci: Mater Med 22: 2781–2789.
- 23. Anselme K (2000) Osteoblast adhesion on biomaterials. Biomaterials 21: 667–681.
- 24. Guleryuz H, Cimenoglu H (2004) Effect of thermal oxidation on corrosion and corrosion-wear behaviour of a Ti-6A1–4V alloy. Biomaterials 25: 3325–3333.
- 25. Ma PX (2008) Biomimetic materials for tissue engineering. Adv Drug Deliv Rev 60: 184–198.
- 26. Zeng HT, Chittur KK, Lacefield WR (1999) Analysis of bovine serum albumin adsorption on calcium phosphate and titanium surfaces. Biomaterials 20: 377–384.
- 27. Sader MS, LeGeros RZ, Soares GA (2009) Human osteoblasts adhesion and proliferation on magnesium-substituted tricalcium phosphate dense tablets. J Mater Sci: Mater Med 20: 521–527.
- 28. Benoit DSW, Schwartz MP, Durney AR, Anseth KS (2008) Small functional groups for controlled differentiation of hydrogel-encapsulated human mesenchymal stem cells. Nat Mater 7: 816–823.
- 29. Malaval L, Modrowski D, Gupta AK, Aubin JE (1994) Cellular expression of bone-related proteins during in vitro osteogenesis in rat bone-marrow stromal cell-cultures. J Cell Physiol 158: 555–572.
- 30. Maddi A, Hai H, Ong ST, Sharp L, Harris M, et al. (2006) Long wave ultrasound may enhance bone regeneration by altering OPG/RANKL ratio in human osteoblast-like cells. Bone 39: 283–288.
- 31. Habibovic P, Barralet JE (2011) Bioinorganics and biomaterials: Bone repair. Acta Biomater 7: 3013–3026.
- 32. Lee NK, Sowa H, Hinoi E, Ferron M, Ahn JD, et al. (2007) Endocrine regulation of energy metabolism by the skeleton. Cell 130: 456–469.
- 33. Chesters JK (1998) Molecular biological approaches to nutrient-gene interactions. Proc Nutr Soc 57: 249–256.
- 34. Cousins RJ (1998) A role of zinc in the regulation of gene expression. Proc Nutr Soc 57: 307–311.
- 35. Ito A, Kawamura H, Otsuka M, Ikeuchi M, Ohgushi H, et al. (2002) Zinc-releasing calcium phosphate for stimulating bone formation. Mater Sci Eng C-Biomimetic Supramol Syst 22: 21–25.
- 36. Kawamura H, Ito A, Miyakawa S, Layrolle P, Ojima K, et al. (2000) Stimulatory effect of zinc-releasing calcium phosphate implant on bone formation in rabbit femora. J Biomed Mater Res 50: 184–190.
- 37. Ito A, Otsuka M, Kawamura H, Ikeuchi M, Ohgushi H, et al. (2005) Zinc-containing tricalcium phosphate and related materials for promoting bone formation. Curr Appl Phys 5: 402–406.
- 38. Kwun IS, Cho YE, Lomeda RAR, Shin HI, Choi JY, et al. (2010) Zinc deficiency suppresses matrix mineralization and retards osteogenesis transiently with catch-up possibly through Runx 2 modulation. Bone 46: 732–741.
- 39. Stein GS, Lian JB, Owen TA (1990) Relationship of cell growth to the regulation of tissue-specific gene expression during osteoblast differentiation. FASEB J 4: 3111–3123.
- 40. Franceschi RT, Iyer BS (1992) Relationship between collagen synthesis and expression of the osteoblast phenotype in MC3T3-E1 cells. J Bone Miner Res 7: 235–246.
- 41. Ehara A, Ogata K, Imazato S, Ebisu S, Nakano T, et al. (2003) Effects of α-TCP and TetCP on MC3T3-E1 proliferation, differentiation and mineralization. Biomaterials 24: 831–836.
- 42. Kimelman N, Pelled G, Helm GA, Huard J, Schwarz EM, et al. (2007) Review: Gene and stem cell based therapeutics for bone regeneration and repair. Tissue Eng 13: 1135–1150.
- 43. Levenberg S, Huang NF, Lavik E, Rogers AB, Itskovitz Eldor J, et al. (2003) Differentiation of human embryonic stem cells on three-dimensional polymer scaffolds. Proc Natl Acad Sci USA 100: 12741–12746.
- 44. Richardson TP, Peters MC, Ennett AB, Mooney DJ (2001) Polymeric system for dual growth factor delivery. Nat Biotechnol 19: 1029–1034.
- 45. Takahashi T, Ogasawara T, Kishimoto J, Liu GY, Asato H, et al. (2005) Synergistic effects of FGF-2 with insulin or IGF-I on the proliferation of human auricular chondrocytes. Cell Transplant 14: 683–693.
- 46. Canalis E, Rydziel S, Delany AM, Varghese S, Jeffrey JJ (1995) Insulin-like growth-factors inhibit interstitial collagenase synthesis in bone cell-cultures. Endocrinology 136: 1348–1354.
- 47. Hill PA, Reynolds JJ, Meikle MC (1995) Osteoblasts mediate insulin-like growth-factor-I and growth-factor-II stimulation of osteoclast formation and function. Endocrinology 136: 124–131.
- 48. Fox SW, Lovibond AC (2005) Current insights into the role of transforming growth factor-β in bone resorption. Mol Cell Endocrinol 243: 19–26.
- 49. Janssens K, ten Dijke P, Janssens S, Van Hul W (2005) Transforming growth factor-β1 to the bone. Endocr Rev 26: 743–774.
- 50. Yamaguchi M, Hashizume M (1994) Effect of β-alanyl-L-histidinato zinc on protein-components in osteoblastic MC3T3-El cells increase in osteocalcin, insulin-like growth-factor-I and transforming growth-factor-β. Mol Cell Biochem 136: 163–169.
- 51. Zreiqat H, Ramaswamy Y, Wu CT, Paschalidis A, Lu ZF, et al. (2010) The incorporation of strontium and zinc into a calcium-silicon ceramic for bone tissue engineering. Biomaterials 31: 3175–3184.